- By
**Rita** - Follow User

- 321 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about 'Aggregate Properties HMA' - Rita

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

### Concensus Aggregate Properties

- All matter has mass and occupies space.
- Volumetrics are the relationships between mass and volume
- Superpave mix design based on aggregate and mixture volumetrics

NCAT

Volume

Mass Water

Volume

Specific Gravity, G

- Ratio of the mass to volume of an object to that of water at the same temperature

NCAT

- Density is the unit weight of a material
- lb/ft3 or kg/m3
- Unit weight = gw G

gw = 1.000 g/cm3

gw = 62.4 lb/ft3

gw = 1000 kg/m3

- Bulk density means sample contains more than one mass and/or volume

NCAT

Mass, oven dry

Surface Voids

Gsb =

Vol of agg, + surface voids

Vol. of water-perm. voids

NCAT

Mass, oven dry agg + mass water

Gs, ssd =

Vol of agg, + surface voids

Vol. of water-perm. voids

Surface Voids

NCAT

Phase: a change in state (e.g. solid, liquid, gas)

V = (mass) / (Gsgw)

Mass (Weight)

Volume

Water permeable voids

Aggregate

Solids

NCAT

Specific Gravity Tests for Aggregates

- Two tests are needed
- Coarse aggregate (retained on the 4.75 mm sieve)
- Fine aggregate (passing the 4.75 mm sieve)

NCAT

Coarse Aggregate Specific Gravity

- ASTM C127
- Dry aggregate
- Soak in water for 24 hours
- Decant water
- Use pre-dampened towel to get SSD condition
- Determine mass of SSD aggregate in bucket
- Determine mass under water
- Dry to constant mass
- Determine oven dry mass

NCAT

Coarse Aggregate Specific GravityCalculations

- Gsb = A / (B - C)
- A = mass oven dry
- B = mass SSD
- C = mass under water
- Gs,SSD = B / (B - C)
- Gsa = A / (A - C)
- Water absorption capacity, %
- Absorption % = [(B - A) / A] * 100

NCAT

Fine Aggregate Specific Gravity

- ASTM C128
- Dry aggregate
- Soak in water for 24 hours
- Spread out and dry to SSD
- Add 500 g of SSD aggregate to pycnometer of known volume
- Pre-filled with some water
- Add more water and agitate until air bubble have been removed
- Fill to line and determine the mass of the pycnometer, aggregate and water
- Empty aggregate into pan and dry to constant mass
- Determine oven dry mass

NCAT

Fine Aggregate Specific GravityCalculations

- Gsb = A / (B + S - C)
- A = mass oven dry
- B = mass of pycnometer filled with water
- C = mass pycnometer, SSD aggregate and water
- S = mass SSD aggregate
- Gs,SSD = S / (B + S - C)
- Gsa = A / (B + A - C)
- Water absorption capacity, %
- Absorption % = [(S - A) / A] * 100

NCAT

Coarse Aggregate Particle Shape

% Crushed Faces

Flat and Elongated

Fine Aggregate Particle Shape

Clay Content

** Determined for the blended aggregate gradation **

NCAT

Percent Crushed Fragments in Gravels

- Quarried materials always 100% crushed
- Minimum values depended upon traffic level and layer (lift)
- Defined as % mass with one or more fractured faces

NCAT

Millions of ESALs < 100 mm > 100 mm

< 0.3

< 1

< 3

< 10

< 30

< 100

100

--/--

--/--

50/--

60/--

80/75

95/90

100/100

55/--

65/--

75/--

85/80

95/90

100/100

100/100

Coarse Aggregate Angularity CriteriaFirst number denotes % with one or more fractured faces

Second number denotes % with two or more fractured faces

NCAT

Flat and Elongated Particles

- ASTM D4791
- Flat
- Elongated
- Total flat and elongated
- Superpave
- Flat and Elongated
- Maximum to minimum dimension
- 5:1
- 3:1
- 2:1

NCAT

Flat and Elongated Criteria

Traffic Maximum, Percent

Millions of ESALs

< 0.3

< 1

< 3

< 10

< 30

< 100

100

--

--

10

10

10

10

10

NCAT

(Uncompacted Void Content of Fine Aggregate)

* Fine aggregate at a specified gradation is allowed to flow freely into a 100 cm3 cylinder.

*Knowing the specific gravity of the aggregate, the voids between aggregate particles can be determined

* The more angular the aggregate, the higher the void content

NCAT

Millions of ESALs < 100 mm > 100mm

< 0.3

< 1

< 3

< 10

< 30

< 100

100

--

--

40

40

40

45

45

--

40

40

45

45

45

45

Fine Aggregate Angularity CriteriaNCAT

(Sand Equivalent Test)

* ASHTO T176, ASTM D2419

- Used to estimate the relative proportions

of fine agg. and clay-like or plastic fines

and dust.

Flocculating Solution

Suspended

Clay

Clay Reading

Sand Reading

SE =

Clay Reading

Sand

Sedimented

Aggregate

Reading

*100

NCAT

Clay Content Criteria

Traffic Sand Equivalent

Millions of ESALs Minimum, Percent

< 0.3

< 1

< 3

< 10

< 30

< 100

100

40

40

40

45

45

50

50

NCAT

Questions - ?

NCAT

Download Presentation

Connecting to Server..